Effect of cobalt chloride (co cl2) on the electrical and optical
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201347Effect of cobalt chloride (CoCl2) on the electrical and opticalProperties of (PVA-PVP-CoCl2) filmsRaya Ali Abid, Majeed Ali HabebBabylon University, College of Education for pure science Department of Physics, IraqE-mail:email@example.comE-mail:firstname.lastname@example.orgAbstractIn this research, many samples have been prepared by adding CoCl2 to the poly vinyl alcohol and poly vinylpyrrolidon with different weight percentages (o, 3, 6 and 9) wt%.The effect of cobalt chloride concentration onthe D.C electrical properties have been investigated. Results showed that the D.C electrical conductivity of suchcomposites increased with increasing of weight percentages of CoCl2, and the activation energy changed withincreasing of filler concentration, as well as the effect of addition cobalt chloride on optical properties of polyvinyl alcohol and poly vinyl pyrrolidon have been studied. The absorbance has been recorded in the wavelength(200-1100) nm, also the absorption coefficient, real and imaginary dielectric constant, energy gap, extinctioncoefficient and refractive index have been determined.Keywords: electrical properties, optical properties, (PVA-PVP) composites, cobalt chloride.IntroductionAlthough many people probably do not realize it, everyone is familiar with polymers. They are all around usin everyday use, in rubber, plastics, resins and in adhesives and adhesive tapes, and their common structuralfeature is the presence of long covalently bonded chains of atoms. They are an extraordinarily versatile class ofmaterials, with properties of a given type often having enormously different values for different polymers andeven sometimes for the same polymer in different physical states. An even greater range of values is availablefor the electrical conductivity of polymers: the best insulating polymer may have a conductivity as low as 10-18 -1m-1, whereas a sample of poly acetylene doped with a few percent of a suitable donor may have aconductivity of 104 -1m-1, a factor of 1022higher. Poly (vinyl alcohol) (PVA), a polyhydroxy polymer, is thelargest, synthetic, water-soluble polymer produced in the world based on volume. It is produced commerciallyby the hydrolysis of poly (vinyl acetate) (PVAC) . Polyvinyl alcohol has excellent film forming, emulsifying,and adhesive properties. It is also resistant to oil, grease and solvent. PVA is odorless and nontoxic, as well ashas high oxygen and aroma barrier properties  PVP is a white ,hygroscopic powder with a weakcharacteristic order .in contrast to most polymers ,it is readily soluble in water and a large number of organicsolvents , such as alcohols ,amines , acids ,chlorinated hydrocarbons , amides and lactase .Experimental workThe samples have been prepared by casting method. The materials used in this work are polyvinyl alcoholand poly vinyl pyrrolidon with CoCl2.The weight percentages of CoCl2 are (3, 6 and 9) wt%. The resistivity wasrecorded by temperature from (50 to 90)0C by using keithley electrometer type (616 C).The volume electricalconductivity defined by: =1/p =1/RA …………………..(1)A=guard electrode effective area.R=volume resistanceL=average thicknessThe activation energy was calculated using equation:σ = σo exp(-Ea / kBT) ………………..(2)σ = electrical conductivity at T temperatureσo= electrical conductivity at absolute zero of temperature.KB = Boltzmann constant and Eact.= Activation EnergyThe absorption spectra of (PVA-PVP-CoCl2 ) composites have been recording in the length range (200-1100)nm by using UV spectrophotometer (UV-1800) ,the absorption coefficient(α) was calculated from thefollowing equation: α= 2.303 A/d .………………(3)Where A is absorption and d is the sample thicknessThe optical energy gap has been calculated by using this equation αhf= B (hf –Eg)r..…..………….(4)
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201348Where hf is the energy of photon, B is proportionality constant and Eg is optical energy gap.The extinction coefficient (k) is directly proportional to the absorption coefficient (α): k=αλ/4π .…………………(5)Where λ is the wavelength of light.The refractive index has been calculated by using this equation n= [4R/(R-1)2- (R+1/R-1)]1/2...……… ……….(6)The real and imaginary part of dielectric constants have been determined from this equation:[11 ]ε1=n2-k2.......................... (7)ε2=2nk ..……………… (8)Results and DiscussionFigure (1) shows the volume electrical conductivity for (PVA-PVP-CoCl2) composites as a function of cobaltchloride concentration. From this figure we can see that the electrical conductivity is increased with theincreasing of the concentration of cobalt chloride composites. This behavior attributed to the increase of the ionscharge carriers [12,13].Figure (2) shows the variation of electrical conductivity of (PVA-PVP-CoCl2) withtemperature. The volume electrical conductivity increases with increasing of temperature this is means that thesematerials have resistance of negative thermal coefficient (i.e. that resistance decrease with temperatureincreased).The explanation of this behavior is the polymeric chains and impurity ions act as traps to make chargecarriers moving by hopping process. The conductivity of all samples will increase because of the increasingcharge carriers and its movement. , these results are similar to the results reached by the researchers in thisbehavior Figure (1): Variation of D.C electrical conductivity with CoCl2 wt% concentration.Figure (2): Variation of D.C electrical conductivity with temperature.Figure (3) show that the variation of Ln D.C electrical conductivity with inverted absolute temperature ofcomposites, the activation energy was determined from equation (2).The activation energy has high values at low
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201349concentration while at high concentration it has low values, these due to increase the local levels in the distancebetween conduction band and valence band ,this is consistent with the findings of the researchers .Thedecrease in activation energy with increasing (CoCl2) concentration shown in figure (4).Figure (3): Variation of D.C electrical conductivity with reciprocal absolute temperature of composites.Figure (4): Variation activation energy with CoCl2 concentration.The relationship between the absorbance and wavelength of the incident light for (PVA-PVP-CoCl2)composites at room temperature shown in figure (5). From this figure note that intensity of the peak increases asa result of increasing concentration of CoCl2 and no shift in the peak position. The increase of absorbance withthe increase of weight percentage of the CoCl2, this is due to absorb the incident light by free electrons .Figure (5): Variation between Absorbance and wavelength of composites.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201350Figure (6) shows the relation between the absorption coefficient and photon energy of the (PVA-PVP-CoCl2) composites. From this figure it note that the absorption coefficient dependent on the photon energy,where the absorption is little at low energy this is means that the possibility of electron transition is little becausethe energy of the incident photon is notice sufficient to move the electron from the valance band to theconduction band. At high energies the absorption coefficient assists in figuring out the nature of electrontransition when the values of the absorption coefficient is high (α >104) cm-1it is expected that direct transitionof electron occur on the other hand when the values of absorption coefficient is low (α <10-4) cm-1it is expectedthat indirect transition of electron occur .Figure (6): The absorption coefficient with various photon energy of composites.The relation between (αhf) 1/2(cm-1.eV)1/2and photon energy of composites shown in figure (7) from thisfigure we note that the value of optical energy gap decrease by increasing of weight percentage of cocl2,also thetransition which occurs in the samples is allowed indirect transition as shown in table (1).This behaviorattributed to the fact that composites are of heterogeneous type (i.e. the electronic conduction depends on addedimpurities), the increase of the added rate provides paths in the polymer which facilitate the crossing of electronfrom the valence band to the conduction band, this explains the decrease of energy gap with the increase of theadded salt .Table (1) Show values of energy gap for indirect transition (allowed, forbidden) of(PVA –PVP-CoCl2) compositesSampleThe values of energy gap for the indirect transition (eV)allowed forbiddenpure 4.85 4.63wt% 4.7 4.46wt% 4.55 4.29wt% 4.5 4.1Figure (8) shows the relationship between (αhf)1/3(cm-1.eV)1/3and photon energy of composites ,we can seefrom this figure the value of forbidden energy gap decreases by increasing weight percentage of CoCl2,as well asthis value of forbidden indirect transition is less than the one value which is represent allowed indirecttransition.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201351Figure (7): The relationship between (αhυ)1/2(eV.cm-1)1/2and photon energy of composites.Figure (8): The relationship between (αhυ)1/3(eV.cm-1)1/3and photon energy.Figure (9) show the relation between refractive index and photon energy for PVA-PVP-CoCl2 composites.From this figure we find out the refractive index increase with increasing CoCl2 concentration because ofincreasing in density composites. In the ultraviolet region we note that a high values of the refractive indexbecause of the little transmittance in this region, but in the visible region note that low values because of the hightransmittance in this region.The variation between extinction coefficient of (PVA-PVP-CoCl2) compositeswith various photon energy as shown in figure (10). This figure shows that the extinction coefficient has lowvalues at (UV-region) and with little concentration as well as it is increased with increasing additiveconcentrations of CoCl2 because of increasing in absorption coefficient, but at visible region we note that theextinction coefficient is very low because of the low absorption at this region .Figure (9): The variation between refractive index and photon energy of composites.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201352Figure (10): The relationship between extinction coefficient and photon energy of composites.The figures (11,12) show that variation between (real and imaginary) parts of dielectric constants. It isconcluded that the variation of ε1 mainly depends on (n2) because of small values of (K2), while ε2 mainlydepends on the (K) values which are related to the variation of absorption coefficients.Figure (11): The variation of real part of dielectric constant with photon energy of composites.Figure (12): The variation of imaginary part of dielectric constant with photon energy of composites.Conclusions1- D.C electrical conductivity for (PVA-PVP-CoCl2) composites increased with increasing of temperature andCoCl2 wt.% concentration.2- Activation energy of PVA-PVP-CoCl2 composites decreases with increasing of the CoCl2 concentration.3- The absorption coefficient for all PVA-PVP-CoCl2 samples increases with increasing of CoCl2 wt.%concentration.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 2013534- The energy gap of indirect transition decreases with increasing of CoCl2 wt.% concentration.5- Extinction coefficient, refractive index and dielectric constant (real and imaginary) increased with increasingof concentration.References I. David, "Introduction to physical polymer", new Cambridge university press, 2002. B.L. Lopez, A.I. Mejia, L. Sierra, "Biodegrade ability of polyvinyl alcohol", Polymer Engineeringand Science, Vol.39, 8, pp.1346-1352, 1999. V. Sedlarik, N. Saha, I. Kuritka, P. Saha, "Environmentally friendly biocomposite based on wasteof the dairy industry and polyvinyl alcohol", Journal of Applied Polymer Science, Vol. 106, 3,pp.1869-1879, 2007. A. H. Nomani, "study the effect of gamma rays on some physical properties of the polymerhydroxyethyl", cellulose and cellulose instance, M.Sc Thesis, University of Babylon-Faculty ofScience, 2000. K. Ramaiah and V. Raja, "Materials in Electronics", J. Materials Science, Vol.10, No.2, pp.145-149, 1999. N. F. Mott and E.A. Davis, "Electronic Processes in Non Crystalline Materials", Calderon PressOxford, 1979. C. Mwolfe, N. Holouyak and G.B. Stillman, "Physical properties of Semiconduc-tor", prenticeHall, New York, 1989. G. Sami Salman, "optical and structural properties of SnO2 membranes Tinged by fluorosis andgamma-ray irradiated", Master, Faculty of Sciences, University of Baghdad, 2005. R Tintu, K. Saurav, K. Sulakshna, Vpn. Nampoori, Pradha krishnan and Sheenuthomas,"Ge28Se60Sb12 /PVA composite films for photonic application", Journal of Non-Oxide Glasses,Vol. 2, No 4, pp.167-174, 2010. B. H. F. AL-Khayat and F. A. Awni, J. Am. Ceram. Soc. Bull., 64(4), pp598-601, 1985. M. Revanasiddappa, S.C. Raghavendra, S. Khasim and T.K. Vishnuvardhan, J. Bull. Koreanchem., Soc. Vol. 28 , No.7, pp.1104-1108, 2007. T. Yao and S. Matsuoko, J. Appl. Phys, Lett., Vol.43, No.5, 1983. S. R. Elliott, Phil. Mag., B, Vol.37, No.5, p.553, 1978. J. Wiley, "Effect of Metal concentration on the Electrical conductivity and some mechanicalproperties of poly methyl methacrylate-Copper composites", J. of Appl. Poly., Vol.20, 1976. E.A. Stefanescu, X. Tan, Z. Lin, N. Bowler and M. R. Kessler, "Multifunctional fiberglass-reinforced PMMA-BaTiO3 structural/dielectric Composites Polymer", 52 pp.2016-2024, 2011. O. A. Abdul-Hussein, "study the electrical properties of poly methyl methacry-late Tinged byhalogenated sodium salts", M.Sc thesis, Faculty of Education, University of Mustansiriya, 2006. P.U. Asogwa, "Band gap shift and optical characterization of PVA Capped PbO thin films: Effectof thermal annealing", Chalcogenide Letters ,Vol.8, No.3, pp.163-170, 2011. G. Pinto and Abdel-Karim Maaroufi, "Critical filler concentration for electro conductive polymercomposites", Society of Plastics Engineers (SPE), 10.1002/ spepro.003521, 2011. K. Gabur , "preparation and study the electrical and optical properties of (PS-Ni) Composites",M.Sc Thesis, Babylon University, College of Science, 2010. M. Dahshan, "Introduction to material science and Engineering", 2nd ed., 2002. M. K. Mahsan1, C.K. Sheng1, M.I. Isa1, E. Ghapur E. Ali 1, M. H. Razali, "Structural andPhysical Properties of PVA/TiO2 Composite", Malaysia Polymer International Conference,pp.486-495, 2009. K. Bula1, T. Jesionowski and S. Borysiak, Proceedings of the Conference of MultiphasePolymers and Polymer Composites: From Nan scale to Macro Composites, Paris-Est, CreteilUniversity, June, France, 2011.